DOI: 10.1007/s00339-004-2618-x Appl. Phys. A 79, 1019–1022 (2004)
Materials Science & Processing
Applied Physics A
d. bleineru p. gasser
Structural features of laser ablation particulate
from Si target, as revealed by focused
ion beam technology
EMPA – Swiss Federal Laboratories for Materials Testing and Research, Ueberlandstrasse 129, 8600 Duebendorf, Switzerland
Received: 1 October 2003/Accepted: 22 January 2004 Published online: 26 July 2004 • © Springer-Verlag 2004 ABSTRACTHeterogeneity in laser-induced particle structures was investigated by scanning electron microscopy (SEM) and transmission electron microscopy (TEM) of individual particles micro-machined using focused ion beam (FIB). The primary particle size distribution spanned over three orders of magni-tude, i.e., in the range 10 nm–10µm with few larger secondary objects. The particulate larger than 0.5 µm often resulted from particle–particle aggregation, mostly upon a spherical core, seldom in chain-like structures. The core of these fractal aggre-gates was found to be polycrystalline. The heterogeneity of the particles with respect to structure and chemistry is surely of im-portance for elemental analysis using laser ablation as sample introduction technique.
PACS39.30.+w; 61.46.+w; 81.20.Rg
Laser ablation inductively coupled plasma mass spectrometry (LA–ICP MS) is based on the analytical infor-mation contained in and transported by laser-induced particles to the plasma mass spectrometer. Many researchers have ded-icated efforts to investigate the influence of several operat-ing parameters on the analytical results, like for instance the wavelength, pulse width, beam profile, cell geometry and how to optimise them [1–10]. The mechanism of formation and transport of the particles, the size distribution and the trans-port efficiency as well as the efficiency of thermal decompos-ition in the ICP are still debated.
Si wafers are technologically relevant samples and the possibility to have access to the spatial distribution of trace elements in them using LA – ICPMS is the driving force of this study. The aim of this work was to investigate the struc-ture of laser ablated particles at relatively high fluence, and the particle behaviour inside the ablation chamber.
Si wafer with a surface 100 nm multi-elemental layer (i.e. Ba, Sr, Ti, Pt, Rh) was ablated for 30 s, using an in-house modified PE 320 Nd: YAG laser sampler, oper-ated at the frequency-quadrupled wavelength (266 nm), with u Fax: +41-1/821-62-44, E-mail: firstname.lastname@example.org
a pulse energy of 4± 0.2 mJ resulting in a fluence of ap-prox. 50 J/cm2. Argon and helium were used as carrier gases at a flow of 0.9 l/min through the chamber (standard op-erating conditions for ICP MS analysis). The sample was micro-machined with a Strata DB 235 dual beam (DB) fo-cused ion beam (FIB) workstation (‘FEI company, USA’) that incorporates a FIB and a scanning electron microscope (SEM) column tilted to each other at an angle of 52◦. The FIB column is adjustable from 1 pA to 20 000 pA at 30 kV with a specified resolution of 7 nm, as given by the manufac-turer. The instrument is equipped with four secondary electron and ion detectors. The workstation has a digital patterning generator and four gas injection systems (GIS) for deposi-tion and specific etching processes. The transmission electron microscope (TEM) specimens were prepared by milling an electron-transparent sample (e.g., 20µm long, 5 µm wide and 100 nmthick) out of a bulk sample including the particle of interest. A Philips CM 30 TEM operated at an acceleration voltage at 200 kV was used to study the microstructure. 3 Results and discussion
Figure 1 shows a survey of the ablated particles around the ablation site. The ablation crater is characterised
FIGURE 1 Top-view of one ablation crater. Hydrodynamic instability favours the elevation of the crater rim. Ablation products are distributed around the pit. In proximity to the irradiated spot the surface layer has been thermally mobilised
1020 Applied Physics A – Materials Science & Processing by a pronounced wall of 40µm height (He) or 50 µm (Ar), induced by extensive hydrodynamic instability of the sam-ple at the spot rim. The dimensions of the ejected particulate span over three orders of magnitude, from a few tens of nm up to 10µm. Primary particles are mostly well-rounded, and secondary products result from aggregation by deposition of nano-particles upon micro-particles. In Fig. 2a, details of the region close to the crater wall are shown. Particles as large as 9–10µm were observed as individual droplets or frac-tal aggregates. These fracfrac-tal aggregates negatively affect the analytical determination in two ways. Firstly, they are not efficiently transported from the sample chamber to the ICP MS. Secondly, their atomisation in the plasma source will not be complete, leading to loss of signal. The region close to the crater, directly outside the irradiated spot, experienced thermal stress as shown in Fig. 2b. Here the surface multi-elemental layer has been thermally mobilised, vaporised dur-ing the irradiation across an aureole 10µm wide around the crater. ‘Remote’ sampling, i.e. sample removal not specific to the ablation spot, was a consequence of lateral thermal trans-port, typical of ‘ns’ ablation. The 10µm aureole of thermal stress suggests a “thermal transport” coefficient of approxi-mately 103cm−1, which is several orders of magnitude lower than the absorption coefficient of Si at 266 nm . Figure 2c shows melt droplets as large as 1µm scattered about. These rounded particles adhere firmly to the sample surface or can capture fine particulate from the gas, so inducing losses in the transported ensemble. Depending on the moment of de-position, these spherical particles experience longer or shorter surface accretion by nano-particles deposition. This ageing process contributes to the evolution of the particle outer struc-ture from a smooth surface into a fluffy one. Figure 2c shows primary particles deposited at different times during the ab-lation experiments so that different ageing is translated into different extent of surface growth. This image also allows one
FIGURE 2 Overview of ablation products. See text for description
to rule out the hypothesis that the fluffy structure is due to ther-mal shock of the particles upon cooling. Figure 2d presents a magnification of the external fractal surface of one of these accreted particles whose surface nano-particulate is known to be enriched in volatile elements . On the background the nano-particulate is densely covering the sample surface. The fractal dimension  of aggregated particles was determined to be in the range Df= 1.39 − 1.86, depending on particle ageing.
Figure 3 shows the structure of particles in different am-bient gases, cross-cut using FIB. In Fig. 3a the SEM image was taken after the particle was stabilised to the floor using the GIS, so the outer mass is artificial Pt coating (this is not present in Fig. 3b–d taken in Ar , He, N2 ambient). In LA– ICP MS argon or helium is routinely used as a carrier gas, so there is great interest in the particle characteristics of these gases. For comparison, Fig. 3d shows the particle structure from ablation in nitrogen. The particle in air is characterised by a rounded core and an outer fluffy corona aftergrowth. The core is oblate due to the impact onto the surface. After settling, nano-particulate present in the ablation chamber volume de-posited progressively onto the surface. The outer corona thins out toward the floor where it is totally absent. The diffusion in the gas volume influences the particle concentration profile in the ablation cell and so also the growth rate of the surfaces. High growth rates are obtained for high concentration regions. In recent works [10, 14] it was shown that particle concentra-tion inside the cell volume is more uniform in helium ambient than in argon, due to physical properties of the gases. Among the two, Ar enhances particle-wall reaction. Thus, diffusion-limited aggregation  leads to the fractal aggregates with uniform corona for the ablation in helium. A thickness gradi-ent characterises the aggregation in argon as a consequence of particle concentration gradient toward the walls. In both cases, in proximity to the sample surface the corona is not
BLEINERet al. Structural features of laser ablation particulate from Si target, as revealed by focused ion beam technology 1021
FIGURE 3 FIB cross-section of particles ablated in dif-ferent ambient gases. a air, b argon, c helium, d nitrogen
FIGURE 4 Radial thickness of the sheath layer (corona) as a function of elevation from the floor in argon and helium
developed, due to this ‘wall effect’ exerted by the sample sur-face on the aerosol concentration. Figure 4 shows the radial thickness of the corona at several elevations above the sample surface, in argon and helium, showing that in argon a factor of three larger gradient of the particle concentration profile is present with respect to helium.
The observations made would suggest that particle loss in-side the sample chamber is a systematic phenomenon. Large cells enhance the loss of particles and deplete the signal in-tensity. Since particle transport efficiency is a size-dependent process , and since nano and micro particles are chemi-cally heterogeneous, then analyte-dependent signal deviation is induced by particle fractionation.
Figure 5 shows a particle sliced with FIB into a 100-nm-thin lamella, and this 100-nm-thin lamella was then used for
transmis-FIGURE 5 TEM lamella of a particle produced in helium that has trapped a gas bubble during settling. See text for description
sion electron microscopy (TEM) [17–19]. In order to stabilize the particle to the sample floor, GIS was used (black embed-ding mass). The crystallographic characteristics of the par-ticle have been investigated by selected area electron diffrac-tion (SAED) patterns obtained at different locadiffrac-tion on the lamella. Multiple crystals could be recognized in the par-ticle core, which are however different orientations of the same lattice. A crystallization sequence, from a precocious euhedral individual to a tardive “filler” could be identified
1022 Applied Physics A – Materials Science & Processing from geometric relations of the crystal edges. Furthermore, the lattice of the tardive crystal is distorted as indicated by an “optical wave” of the reflexes obtained rotating the angle of the lamella relative to the electron beam. This indicates that heat removal was more rapid on one part than on an-other, which could be caused by the flow direction of the gas in the chamber. The texture of the corona would sug-gest that the gas was flowing from right to left in Fig. 5, because on the upstream side the corona is uniform whereas on the downstream side turbulence has produced the irregular growth.
Large variability in the primary mechanism of laser ablation particle formation and heterogeneity in the shape as well as in the composition were observed in the case of sil-icon. Post-sampling nano-micro particle aggregation led to secondary particulate whose outer surface growth rate is sig-nificantly influenced by the ambient gas. Surface development and internal crystalline features of the laser-induced particles were documented. Signal drift in analytical measurement sig-nals is surely influenced by particulate heterogeneity.
ACKNOWLEDGEMENTS U. Klotz is acknowledged for valu-able support with the TEM instrument. U. Sennhauser is acknowledged for permitting access to the instruments in his department. The authors are also grateful to P. Lienemann and M. Trottmann for productive discussions.
H. Vonmont is acknowledged for supporting the post-doc project of one author (Bleiner), with EMPA dossier number 840744.
1 D. Günther, C.A. Heinrich: J. Anal. Atom. Spectrom. 14, 1369 (1999) 2 T.E. Jeffries, S.E. Jackson, H.P. Longerich: J. Anal. Atom. Spectrom. 13,
3 J.J. Gonzalez, S.S. Mao, X.L. Mao, J. Roy, R.E. Russo: J. Anal. Atom. Spectrom. 17, 1108 (2002)
4 R.E. Russo, X.L. Mao, S.S. Mao, J.J. Gonzalez: J. Anal. Atom. Spectrom 17, 1072 (2002)
5 V. Margetic, M. Bolshov, A. Stockhaus, K. Niemax, R. Hergenroeder: J. Anal. Atom. Spectrom. 16, 616 (2001)
6 L. St-Onge: J. Anal. Atom. Spectrom 17, 1083 (2002)
7 M. Guillong, I. Horn, D. Günther: J. Anal. Atom. Spectrom. 18, 1224 (2003)
8 I. Horn, D. Günther: Appl. Surf. Sci. 207, 144 (2003)
9 M. Guillong, D. Guenther: J. Anal. At. Spectrom. 17, 831 (2002) 10 D. Bleiner: ETH Dissertation 14 665
11 C. Eisele, C.E. Nebel, M. Stutzmann: Solid-State Phenom. 80–81, 205 (2001)
12 P.M. Outridge, W. Doherty, D.C. Gregoire: Spectrochim. Acta, Part B 51, 1451 (1997)
13 M. Ullmann, S.K. Friedlander, A. Schmidt-Ott: J. Nanopart. Res. 4, 499 (2002)
14 D. Bleiner, P. Lienemann, M. Trottmann, A. Ulrich: Canad. J. Anal. Sci. Spect., Special issue ICASS (2003)
15 T.A. Witten, J. Sander, L.M. Sander: Phys. Rev. Lett. 47, 1400 (1981) 16 M.A. Gilbertson, I. Eanes: Powder Technol. 131, 197 (2003) 17 A.E.M. De Veirman: Mater. Sci. Eng., B 102, 63 (2003)
18 J.C. Reiner, P. Gasser, U. Sennhauser: Microel. Reliab. 42, 1753 (2002) 19 Ph. Gasser, U. Klotz, F.A. Kahlid, O. Beffort: Microsc. Microanal. 10, 1